Graphene is a leading contender for the next-generation electronic devices. We report a method to produce graphene membranes in the solution phase using polymeric imidazolium salts as a transferring medium. Graphene membranes were reduced from graphene oxides by hydrazine in the presence of the polyelectrolyte which is found to be a stable and homogeneous dispersion for the resulting graphene in the aqueous solution. A simple device with gold contacts on both sides was fabricated in order to observe the electronic properties.
The unique physical, electronic, and optical properties of graphene have been reported many times [1–4] and promise a wide variety of applications. Different methods have been adopted for obtaining graphene, e.g., mechanical exfoliation of graphite , epitaxial growth , and chemical exfoliation in different solutions [3, 7–9]. A very promising route for the bulk production of the graphene sheets can be chemical reduction and dispersion of graphene in aqueous solutions.
Two steps are involved in making water dispersible graphene: (1) first chemical oxidation of graphite to hydrophilic graphite oxide and (2) exfoliating it into graphene oxide (GO) sheets in aqueous solution. GO sheets are graphene sheets having oxygen functional groups. These GO sheets are prevented from agglomeration by electrostatic repulsion alone . The insulating GO can easily be reduced to highly conducting graphene by hydrazine reduction. However, the reduction of GO soon leads to agglomeration, while a stable dispersion is key to the possibility of large-scale processing. Polymeric imidazolium salts can be a good way to form a stable dispersion of graphene.
Organic salts based on the imidazolium moiety are an interesting class of ions. Low molecular weight imidazolium salts can have a low melting point and are then termed ionic liquids (ILs). Thus, ILs are molten salts at the room temperature and consist of bulky organic cations paired with organic or inorganic anions. Imidazolium ionic liquids have many advantageous properties, such as no flammability, a wide electrochemical window, high thermal stability, wide liquid range, and very small vapor pressure . They are also known to interact strongly with the basal plane of graphite and graphene. Polymeric imidazolium salts would therefore be interesting to explore as dispersing agents for graphene.
Graphene oxide was prepared by the modified Hummer's method [12, 13]. The graphite flakes (PN 332461, 4 g; Sigma Aldrich, Sigma-Aldrich Sweden AB,) were first put in H2SO4 (98%, 12 mL) and kept at 80°C for 5 h. The resulting solution was cooled down to room temperature. Mild sonication was performed in a water bath for 2 h to further delaminate graphite into a few micron flakes. Sonication time and power are very critical as they define the size of the resulting graphene oxide sheets. Excessive sonication leads to extremely small flakes. Then, the solution was diluted with 0.5 L deionized (DI) water and left overnight. The solution was filtered by Nylon Millipore™ filters (Billerica, MA 01821). The resulting powder was mixed with KMnO4 and H2SO4 and put in a cooling bath under constant stirring for 1.5 h. The solution was diluted with DI water, and 20 mL H2O2 (30%) was added to it.
The supernatant was collected after 12 h and dispersed in dilute HCl in order to remove the metal ion residue and then recovered by centrifugation [12, 13]. Clean GO was again dispersed in water to make a homogeneous dispersion and was centrifuged at 8,000 rpm for 40 min in order to remove the multilayer fragments. We added a polymeric imidazolium molten salt into the aqueous dispersion of GO at a concentrationof 1 mg mL-1 and strongly shook the solution for a few minutes. The imidazolium salt used by us was polyquaternium 16 (PQ-16) sold under the trade name Luviquat Excellence by BASF (Ludwigshafen, Germany), a copolymer with 95% molar of imidazolium chloride and 5% molar of vinylimidazole. Use of this polymeric salt for graphene dispersion is not found in literature. Then, the solution was reduced by hydrazine monohydrate at 90°C for 1 h to obtain a stable dispersion of graphene in aqueous solution.
Results and discussion
This aqueous PQ-graphene dispersion was found to be stable even after 2 months, whereas the reduced GO without the addition of PQ-16 formed agglomerates soon after reduction with hydrazine. Thus, PQ-16 is the main cause of a stable dispersion of graphene membranes in aqueous solution. The underlying mechanism has been affiliated with adsorption of some of the polycations on the surface of the graphene membranes by non-covalent π-π interactions between the imidazolium rings of the salt and graphene, soon after reduction with hydrazine monohydrate. The graphene was deposited onto Si/SiO2 (SiO2 thickness approximately 300 nm) substrates by dip-coating. Schematic of the whole process is shown in Figure 1.
The sample was rinsed with DI water and dried with nitrogen. The dried samples were further treated at 400°C for 2 h in Ar/H2 to further reduce the graphene oxide and also to sublimate the solution residue. The optical microscope images were taken in order to identify graphene . Atomic force microscope measurements were carried out to confirm the presence of single- and few-layer graphene by measuring step height . Graphene shows typical wrinkled structure which is intrinsic to graphene  over relatively large sheet sizes. Very large graphene membranes with sizes around 10 × 10 μm were identified. The size was found to be directly related with sonication power and time. Excessive sonication results in very small graphene sheets, whereas insufficient sonication results in incomplete exfoliation of graphite oxide.
We measured the height profiles of the graphene membranes by atomic force microscopy (AFM) after drop casting them on a relatively flat SiO2/Si substrate. The average thickness of a GO sheet was approximately 1 nm (Figure 2), which was in agreement with the preceding research, confirming that the graphite oxide was completely exfoliated. We observed heights from slightly less than 1 nm to a few nanometers thick. We assigned the sheets with height approximately 1 nm, approximately 1.5 nm, approximately 2 nm, and up to 5 nm to be one-, two-, three-, and few-layered GO sheets, respectively. This was in agreement with the reported AFM results on few-layer graphene sheets [5, 8, 17], where the single-layer graphene is always approximately 1 nm, probably due to different attraction force between AFM tips and graphene as compared to SiO2 and imperfect interface between graphene and SiO2.
AFM image of our chemically reduced GO sheet after addition of PQ-16, deposited on SiO2/Si substrate by drop casting, is shown in Figure 3. The graphite interlayer spacing is about 0.34 nm which should ideally correspond to the thickness of a monolayer graphene. Conversely, the thickness of single PQ-G was determined to be approximately 1.9 nm. If we assume that monolayered PQ-16 covered both sides of graphene sheet with offset face-to-face orientation via π-π interactions (mechanism of stabilization), the estimated distance between PQ and the graphene sheet is approximately 0.35 nm . Accordingly, the average thickness of the graphene sheet in the PQ-G layer can be derived to be around 1.9 nm. This assumption is further supported by Figure 3b, which shows the step height for the region with bilayer graphene. The step height of the graphene-graphene interface was also observed to be approximately 1.9 nm in various measurements.
Transmission electron microscopy (TEM) is also a very important tool for investigating the quality of exfoliated graphene. We dropped a small quantity of the dispersion on the holey carbon grid by pipette and dried the samples. Figure 4a shows bright-field TEM image, Figure 4b shows the high-resolution transmission electron microscope (HRTEM) image of the graphene surface, and Figure 4c depicts the electron diffraction pattern observed from the same area. The analysis of the diffraction intensity ratio was used to confirm the presence of monolayer graphene . We use the Bravais-Miller (hkil) indices to label the peaks corresponding to the graphite reflections taken at normal incidence . After analyzing a large number of TEM images, we were able to conclude that our dispersion contains a very good fraction of monolayer graphene.
We fabricated a bottom-gated graphene field-effect transistor (FET) by putting a monolayer of reduced GO membrane in between thermally evaporated gold electrodes. The channel length between source and drain electrodes was 5 μm. The schematic and the scanning electron microscope (SEM) image of the device are shown in Figure 5. Figure 5c shows the drain current (I d) vs. gate voltage (V g) curve of FET prepared with this reduced monolayer graphene membrane. The FET gate operation exhibits hole conduction behavior. Pure two-dimensional graphene has a zero bandgap that limits its effective application in electronic devices. We believe that this reduced GO from PQ dispersion has a kind of doping effect that makes it more favorable for applications due to its improved electronic properties. There were theoretical simulations [20, 21], which were later confirmed experimentally  that the 100% hydrogenation of freestanding graphene results in a metal to insulator transition. Hydrogenation of graphene on a silicon dioxide (SiO2) substrate has also led to the energy gap opening . Here, we can attribute the deficiency of ambipolar behavior to hole doping caused by residual oxygen functionalities resulting in a p-type behavior and a field-effect response [2, 24]. Thus, chemical functionalization is a possible route to modify the electronic properties of graphene, which can be important for graphene-based nanoelectronics , although there is room for further optimization of the process for improving the properties, in order to make it ideal for industrial level applications.
In summary, we report a method to produce and functionalize graphene membranes in the solution phase using polymeric imidazolium molten salts as a transferring medium. Graphene membranes were reduced from graphene oxide by hydrazine in the presence of a polyelectrolyte which was found to be a very stable dispersion for the graphene membranes in the aqueous solution. The reduced GO membranes were transferred to a SiO2/Si substrate by simple drop casting and were further reduced by annealing in H2/Ar. A simple device with gold contacts on both the sides was fabricated in order to observe the electronic properties. We conclude that chemical functionalization is a possible route to modify and improve the electronic properties of graphene.
Geim AK, Novoselov KS: The rise of graphene. Nat Mater 2007, 6: 183–191. 10.1038/nmat1849
Gilje S, Han S, Wang M, Wang KL, Kaner RB: A chemical route to graphene for device applications. Nano Letters 2007, 7: 3394–3398. 10.1021/nl0717715
Kim T, Lee H, Kim J, Suh KS: Synthesis of phase transferable graphene sheets using ionic liquid polymers. ACS Nano 4: 1612–1618.
Stoller MD, Park S, Zhu Y, An J, Ruoff RS: Graphene-based ultracapacitors. Nano Letters 2008, 8: 3498–3502. 10.1021/nl802558y
Novoselov KS, Geim AK, Morozov SV, Jiang D, Zhang Y, Dubonos SV, Grigorieva IV, Firsov AA: Electric field effect in atomically thin carbon films. Science 2004, 306: 666–669. 10.1126/science.1102896
Hass J, de Heer WA, Conrad EH: The growth and morphology of epitaxial multilayer graphene. Journal of Physics: Condensed Matter 2008, 20: 323202. 10.1088/0953-8984/20/32/323202
Hernandez Y, Nicolosi V, Lotya M, Blighe FM, Sun Z, De S, McGovern IT, Holland B, Byrne M, Gun'Ko YK, Boland JJ, Niraj P, Duesberg G, Krishnamurthy S, Goodhue R, Hutchison J, Scardaci V, Ferrari AC, Coleman JN: High-yield production of graphene by liquid-phase exfoliation of graphite. Nat Nano 2008, 3: 563–568.
Li X, Wang X, Zhang L, Lee S, Dai H: Chemically derived, ultrasmooth graphene nanoribbon semiconductors. Science 2008, 319: 1229–1232. 10.1126/science.1150878
Pichon A: Graphene synthesis: chemical peel. Nat Chem 2008.
Cote LJ, Kim F, Huang J: Langmuir-Blodgett assembly of graphite oxide single layers. Journal of the American Chemical Society 2008, 131: 1043–1049.
Carrión F, Sanes J, Bermúdez M-D, Arribas A: New single-walled carbon nanotubes-ionic liquid lubricant. Application to polycarbonate-stainless steel sliding contact. Tribology Letters 41: 199–207.
Dong X, Su C-Y, Zhang W, Zhao J, Ling Q, Huang W, Chen P, Li L-J: Ultra-large single-layer graphene obtained from solution chemical reduction and its electrical properties. Physical Chemistry Chemical Physics 12: 2164–2169.
Hummers WS, Offeman RE: Preparation of graphitic oxide. Journal of the American Chemical Society 1958, 80: 1339–1339. 10.1021/ja01539a017
Zhou X, Wu T, Ding K, Hu B, Hou M, Han B: Dispersion of graphene sheets in ionic liquid [bmim][PF6] stabilized by an ionic liquid polymer. Chemical Communications 46: 386–388.
Blake P, Hill EW, Neto AHC, Novoselov KS, Jiang D, Yang R, Booth TJ, Geim AK: Making graphene visible. Applied Physics Letters 2007, 91: 063124–063123. 10.1063/1.2768624
Stankovich S, Dikin DA, Dommett GHB, Kohlhaas KM, Zimney EJ, Stach EA, Piner RD, Nguyen ST, Ruoff RS: Graphene-based composite materials. Nature 2006, 442: 282–286. 10.1038/nature04969
Gupta A, Chen G, Joshi P, Tadigadapa S, Eklund : Raman scattering from high-frequency phonons in supported n-graphene layer films. Nano Letters 2006, 6: 2667–2673. 10.1021/nl061420a
Xu Y, Bai H, Lu G, Li C, Shi G: Flexible graphene films via the filtration of water-soluble noncovalent functionalized graphene sheets. Journal of the American Chemical Society 2008, 130: 5856–5857. 10.1021/ja800745y
Meyer JC, Geim AK, Katsnelson MI, Novoselov KS, Obergfell D, Roth S, Girit C, Zettl A: On the roughness of single- and bi-layer graphene membranes. Solid State Communications 2007, 143: 101–109. 10.1016/j.ssc.2007.02.047
Sofo JO, Chaudhari AS, Barber GD: Graphane: a two-dimensional hydrocarbon. Physical Review B 2007, 75: 153401.
Boukhvalov DW, Katsnelson MI, Lichtenstein AI: Hydrogen on graphene: Electronic structure, total energy, structural distortions and magnetism from first-principles calculations. Physical Review B 2008, 77: 035427.
Elias DC, Nair RR, Mohiuddin TMG, Morozov SV, Blake P, Halsall MP, Ferrari AC, Boukhvalov DW, Katsnelson MI, Geim AK, Novoselov KS: Control of graphene's properties by reversible hydrogenation: evidence for graphane. Science 2009, 323: 610–613. 10.1126/science.1167130
Boukhvalov DW, Katsnelson MI: Modeling of epitaxial graphene functionalization. Nanotechnology 2011, 22: 055708. 10.1088/0957-4484/22/5/055708
Allen MJ, Tung VC, Gomez L, Xu Z, Chen L-M, Nelson KS, Zhou C, Kaner RB, Yang Y: Soft transfer printing of chemically converted graphene. Advanced Materials 2009, 21: 2098–102. 10.1002/adma.200803000
Boukhvalov DW, Katsnelson MI: Chemical functionalization of graphene with defects. Nano Letters 2008, 8: 4373–4379. 10.1021/nl802234n
We acknowledge the help of Amir Karim (Acreo Kista) for his technical support in TEM imaging.
The authors declare that they have no competing interests.
All authors contributed equally, read and approved the final manuscript.
About this article
Cite this article
ul Hasan, K., Sandberg, M.O., Nur, O. et al. Polycation stabilization of graphene suspensions. Nanoscale Res Lett 6, 493 (2011). https://doi.org/10.1186/1556-276X-6-493
- Graphene Oxide
- Graphene Sheet
- Graphite Oxide
- Stable Dispersion
- Monolayer Graphene